FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS


 Tamsyn Cross
 1 years ago
 Views:
Transcription
1 FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS Adrian R. Muxworthy* and Andrew P. Roberts School of Ocean and Earth Science, National Oceanography Centre, European Way, University of Southampton, Southampton, SO14 3ZH, UK. *Corresponding author: Tel: +44 () Fax: +44 () Outline: Introduction Measuring and constructing FORC diagrams FORC and Preisach diagrams Characteristic FORC diagrams Further Features of FORC diagrams Applications of the FORC diagram Bibliography 1
2 FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS Introduction In many geomagnetic, geological and environmental magnetic studies, it is important to have reliable methods of characterizing the composition and grain size distribution of magnetic minerals within samples. For example, identification of single domain (SD) magnetic grains is important in absolute paleointensity studies because SD grains produce the most reliable results, while larger multidomain (MD) grains yield the least meaningful results. In paleoclimatic studies, useful environmental information is often revealed by subtle changes in grain size distribution, as revealed by domain state, while the same grain size variations will complicate determination of relative paleointensity from the same sediment. It is therefore crucially important to have reliable methods for determining the magnetic grain size distribution in a wide range of geomagnetic, paleomagnetic and environmental magnetic applications. Determining the composition of magnetic minerals in a rock is relatively straightforward; however, identification of the domain state is more difficult. Conventional methods, such as measurement of magnetic hysteresis, can be powerful, but they can also yield ambiguous results because various combinations of mineral composition, grain size, internal stress and magnetic interactions among the grains can produce the same magnetic behaviour. This is particularly true for the commonly used Day plot (Day et al. 1977), which summarizes the bulk magnetic hysteresis properties by plotting ratios of M rs /M s versus H cr /H c, where M rs is the saturation remanent magnetization, M s is the saturation magnetization, H cr is the coercivity of remanence, and H c is the coercive force (see Hysteresis for a description of how these parameters are determined). For example, numerical studies have shown that magnetostatic interactions among ideal SD grains can cause the bulk hysteresis parameters of samples to plot within the MD region of the Day plot (Muxworthy et al. 23). In an attempt to remove some of the ambiguity inherent to conventional hysteresis measurements, Pike et al. (1999) and Roberts et al. (2) developed a method of mineral and domain state discrimination using a type of hysteresis curve called a firstorder reversal curve (FORC). Measurement of a suite of FORCs provides detailed information from within the major hysteresis loop, which enables determination of the distribution of switching fields and interaction fields for all of the particles that contribute to the hysteresis loop. The ability to measure sufficient FORCs to construct a FORC diagram has only recently become possible with rapid and sensitive vibrating sample magnetometers and alternating gradient magnetometers. 2
3 Measuring and constructing FORC diagrams A FORC is measured by progressively saturating a sample in a field H SAT, decreasing the field to a value H A, reversing the field and sweeping it back to H SAT in a series of regular field steps (H B ) (Fig. 1a). This process is repeated for many values of H A, which yields a series of FORCs, and the measured magnetization M at each step as a function of H A and H B gives M(H A, H B ) (Fig. 1b). M(H A, H B ) can then be plotted as a function of H A and H B in field space (Fig. 1c). The field steps are chosen such that H A and H B are regularly spaced, which means that M(H A, H B ) can be plotted on a regular grid. The FORC distribution (H A, H B ) is defined as the mixed second derivative of the surface shown in Fig. 1c: (H A, H B )  2 M(H A, H B ) / H A H B. (1) When (H A, H B ) is plotted as a contour plot (i.e., as a FORC diagram; Fig. 1d), it is convenient to rotate the axes by changing coordinates from (H A, H B ) to H C = (H B H A )/2 and H U = (H B + H A )/2. As is standard when fitting functions to experimental data, reduction of the effect of noise on FORC distributions is achieved in a piecewise manner. That is, rather than fitting a function to the entire M(H A, H B ) surface and then directly differentiating this surface to determine (H A, H B ), the FORC distribution is determined at each point by fitting a mixed secondorder polynomial of the form a 1 + a 2 H A + a 3 H 2 A + a 4 H B + a 5 H 2 B + a 6 H A H B to a local, moving grid. (H A, H B ) is simply equal to the fitted parameter a 6. As the polynomial is only of second order, it cannot accurately accommodate complex surfaces; however, this will not commonly be a problem for geological or environmental samples, which usually have relatively smooth FORC distributions. The size of the local area is determined by a userdefined smoothing factor (SF), where the size of the grid is simply (2SF+1) 2. SF normally takes values between 2 and 5, although ideally it should be 2. Taking the second derivative in equation (1) magnifies the noise that is inevitably present in the magnetization data. Increasing SF reduces the contribution of noise to the resulting FORC diagram, but it also removes measured data. Simple tests can be conducted to determine suitable smoothing factors for each sample. These tests determine when all of the noise that has been removed by smoothing; if SF is increased above this value, the effect will be only to remove data (Heslop and Muxworthy, 25). A FORC diagram is well described by 114 raw FORCs. Recent improvements in system hardware have made it possible to measure 1 FORCs in approximately 1 hour. The exact time depends on the fieldstep size, the aspect ratio of the FORC diagram, H SAT and the averaging time. The effects of these measurement variables depend as follows. 3
4 (1) The chosen fieldstep size depends ultimately on the mineralogy of the sample under investigation. For a simple SDdominated sample as in Fig. 1d, the main peak of the FORC diagram is directly related to the coercive force H c. It is necessary to choose suitable boundary values for H U and H C to fully depict the FORC distribution. The fieldstep size will be larger for FORC diagrams with larger boundary values, which then increases the measurement time. That is, it will take longer to measure a FORC diagram dominated by high coercivity minerals such as hematite compared to low coercivity minerals such as magnetite. (2) The aspect ratio of the FORC diagram also affects the measurement time. The overall measurement time will decrease as the ratio of the length of the axes, i.e., (H U axis)/(h C axis), increases. A square FORC diagram therefore is optimal in terms of measurement time (but the characteristics of the measured sample should dictate the selected axis lengths). Also, in order to rigorously calculate a FORC distribution, it is necessary to measure points outside the limits of the FORC diagram (depending on the value of SF). This will also (marginally) increase the measurement time. (3) H SAT should be sufficient to magnetically saturate the sample. However, making H SAT unnecessarily large will increase measurement time because of the finite time taken to sweep the magnet down from high values of H SAT. (4) The averaging time is the amount of time taken to measure each data point, and is usually seconds (s). Typically, the averaging time is set to.15 s. Increasing the averaging time increases the total measurement time, but improves signal to noise ratios. In systems that magnetically relax on the same time scale as the averaging time, the averaging time can be critical to the resulting FORC diagram. The averaging time should therefore always be stated in the accompanying text or figure caption. FORC and Preisach diagrams The FORC method originates in the phenomenological PreisachNéel theory of hysteresis (Preisach, 1935; Néel, 1954). There has been much unnecessary confusion in the paleomagnetic community over the relationship between Preisach diagrams and FORC diagrams. Much of this confusion has arisen due to the lack of understanding as to what a Preisach diagram is. Put simply, there a many ways of measuring a Preisach diagram, of which the FORC method is one. 4
5 FORC diagrams are essentially a new welldefined algorithm or method for rapidly generating a particular class of Preisach diagram. Characteristic FORC diagrams Noninteracting SD behaviour To help in the understanding of FORC diagrams, consider a FORC diagram for a SD grain, with uniaxial anisotropy, that is aligned in the direction of the applied field. Such an ideal SD grain will have a perfect square hysteresis loop (Fig. 2a). When plotting raw FORC data for such a particle in nonrotated field space, M(H A, H B ) can take one of two values, i.e., +M s or M s (Fig. 2b). For H A > H SW (where H SW is the switching field), M(H A, H B ) is +M s, for H A < H SW and H B < +H SW, M(H A, H B ) is M s, and for H A < H SW and H B > +H SW, M(H A, H B ) is +M s. On differentiating the surface with respect to H A and H B, only at H A = H B = H SW is M(H A, H B ) nonzero. That is, the FORC distribution should be a perfect delta function, normal to the FORC plane; however, due to the smoothing factor, (H A, H B ) will have finite width (Fig. 2c). An ideal noninteracting uniaxial SD particle with field applied along the easy axis of magnetization will therefore have a FORC distribution that lies at H c = H SW and H u =. For assemblages of randomly orientated, noninteracting, identical, uniaxial SD grains, there are three main features in the FORC diagram (Fig. 3): first, there is a central peak; second, the main peak displays an asymmetric boomerang shape; and third, there is a negative region near the bottom lefthand corner of the FORC diagram. The central peak is due to the switching of the magnetization at H SW. From a more mathematical point of view, the positive peak is associated with the increase in M/ H B with decreasing H A as highlighted in Fig. 3. The lower lefthand arm of the boomerang is related to FORCs near the relatively abrupt positive switching field. The righthand arm of the boomerang is related to more subtle contours, which are due to the FORCs having different return paths, as highlighted in Fig. 3. The shape of the return paths is controlled by the orientation of the grains with respect to the applied field, which results from the fact that the orientation controls the coercivity. Initially, return curve behaviour is dominated by grains oriented ~45 to the field. As H A decreases, grains with orientations closer to 9 and will start contributing to the hysteresis curve, so each time H A is decreased the return path includes grains with slightly differently shaped hysteresis loops. The righthand arm is therefore a result of moving from the return path for a 45 assemblage in the first instance, into the return path for a randomly orientated assemblage. This effect is particularly enhanced for an assemblage of identical grains. The origin of the negative region is related to sections of the 5
6 FORCs where H B < (Newell, 25). As illustrated in Fig. 3, M/ H B decreases with decreasing H A at H B1, which gives rise to negative values for (H A, H B ). The decrease in M/ H B with H A is not as pronounced for H B < ; consequently the negative region is significantly smaller than the large central peak near H B2. If the SD grains have a distribution of switching fields, this causes the FORC diagram to stretch out in the H C direction (Fig. 4). A distribution of coercivities (e.g., Fig. 4) is much more typical of natural samples than an assemblage of identical grains as depicted in Fig. 3. Interacting SD behaviour FORC distributions are highly sensitive to magnetostatic interactions. As a starting point to understanding the contribution of interactions to the FORC diagram, it is simplest to consider Néel s (1954) interpretation of the Preisach (1935) diagram. Néel (1954) showed that for interacting SD grains, H C corresponds to the coercive force of each SD loop in the absence of interactions and that H U is the local interaction field H I. It follows in the PreisachNéel interpretation that (H a, H b ) is the product of two distributions: the coercivity distribution g(h C ) and the interaction field distribution f(h U ). In a simple visualization, when the ideal SD grain in Fig. 2a is affected by magnetic interactions, H I will shift the switching field (Fig. 5a). This asymmetry between the forward and backward switching fields gives rise to spreading in the H U direction on a FORC diagram (Fig. 5b). Micromagnetic models for FORC diagrams have shown that Néel s (1954) approximation is correct for moderately interacting systems, but that it breaks down when the grains are separated by less than a grain width (Muxworthy et al. 24). Highly interacting systems produce FORC diagrams that appear to be essentially the same as those for MD grains (see below and compare Fig. 5 with Pike et al. 21a). MD and pseudosingle domain grains FORC diagrams for large MD grains (Pike et al. 21a) produce a series of contours that run parallel or nearly parallel to the H U axis (Fig. 6a). This spreading of the FORC distribution is essentially the same as for interacting SD grains; instead of the spreading being due to intergrain magnetostatic interaction fields, it is due to internal demagnetizing fields. Pseudosingle domain (PSD) grains display behaviour intermediate between true MD and true SD behaviour (Fig. 6b). That is, they display both the closed peak structures observed for SD grains and the more open contours that become increasingly parallel to the H U axis with coarser grain sizes (Roberts et al. 2). 6
7 Superparamagnetic behaviour Superparamagnetic (SP) grains will only manifest themselves on the FORC diagram if their relaxation time is of the same order as the averaging time (Roberts et al. 2; Pike et al. 21b). If the grains have shorter relaxation times, i.e., H SW, then (H A, H B ) = at all values. SP grains with relaxation times of s have FORC diagrams similar to those for MD grains, i.e., (H A, H B ) plots as a series of contours running almost parallel to the H U axis (Fig. 6c). Although SP behaviour may initially seem similar to MD behaviour, the coercivity spectra of MD and SP samples and the shapes of the FORC distributions can be visually distinguished (Fig. 6a, c). Cooling a sample by a few degrees can also easily enable identification of thermal relaxation. Due to the exponential nature of SD relaxation times, small temperature variations are sufficient to increase relaxation times, which effectively makes the grains thermally stable on the time scale of a measurement. Upon cooling, the FORC diagram for a SP sample would then resemble that of a stable SD sample (cf. Fig. 4). In contrast, FORC diagrams for MD samples would not display such variations with temperature. Further Features of FORC diagrams The H U axis Due to the use of the local grid when calculating a FORC diagram for any value of SF, it is necessary to fit the polynomial surface using points outside the plotted FORC diagram. For the upper, lower and righthand bounds of the FORC diagram, this is readily achievable by simply measuring extra data points. For the H U axis, however, this is not possible. This means that points on the H U axis are not directly measured, and there will be a gap of size 2SF+1 multiplied by the field spacing between (H A, H B ) and the H U axis on the FORC diagram. Three approaches have been made to deal with this problem. (1) Do not plot the FORC distribution for the region where the polynomial cannot be rigorously calculated. This results in a truncated FORC diagram (Fig. 7a). (2) Relax the calculation of (H A, H B ) back on to the H U axis by reducing the smoothing near the H U axis. Such relaxed fit diagrams (Fig. 7b) will produce distortions, which can give misleading results if the field step size is too large, but they have the advantage that it is at least possible to observe low coercivity magnetization components. Such components are usually 7
8 important in natural samples, so relaxing the fit is considered by some workers to be preferable to truncation. (3) Reversibleridge method (Fig. 7c) (Pike, 23). This approach, which has been developed from Preisach theory, accommodates the reversible component of the magnetization data in addition to the irreversible part. With this approach, FORCs are extrapolated beyond H A <, which enables rigorous calculation of (H A, H B ) back on to the H U axis. For SD assemblages this approach can be successful, however, for natural samples containing PSD or MD material the reversible ridge can often swamp the signal from the irreversible component of magnetization. Asymmetry of FORC diagrams The FORC method is a highly asymmetric method of measuring a Preisach diagram. The asymmetry originates from the measurement method in which each FORC starts from a saturated state. In interacting SD and MD systems, this means that there is bias in the magnetostatic interaction and internal demagnetizing fields in the direction of H SAT. The only FORCs that do not contain a history of the initial H SAT state are those that start from a sufficiently large negative H A value that saturates the sample in the opposite direction. Asymmetry is therefore inherent to FORC diagrams. Applications of the FORC diagram FORC diagrams provide much more detailed information about magnetic assemblages than standard hysteresis measurements. Thermal relaxation, variations in domain state and magnetostatic interactions all produce characteristic and distinct manifestations on a FORC diagram. Here we illustrate four applications of FORC diagrams in paleomagnetic and environmental magnetic studies. (1) Unravelling mixed magnetic assemblages. A key problem in many paleomagnetic and environmental studies is identifying and isolating specific minerals and/or grain size distributions within a sample. This can be difficult in mixed samples if the signal from one mineral is magnetically swamped by that of another mineral. FORC diagrams have been shown to be successful at identifying magnetic signals due to minerals with low intrinsic magnetizations when they are present along with more strongly magnetic minerals (Roberts et al. 2; Muxworthy et al. 25). For example, consider a mixture of PSD magnetite and PSD hematite. 8
9 The hysteresis loop in Fig. 8a provides no evidence for the presence of hematite, whereas in the FORC diagram the presence of hematite is clearly visible by the highcoercivity component that extends to high values of H C (Fig. 8b). Although the FORC diagram is more successful than standard magnetic hysteresis measurements at identifying weaker magnetic phases in mixtures with more strongly magnetic phases, there are still concentration thresholds beyond which the magnetic signal of the strongly magnetic phase dominates and the weakly magnetic phase is no longer detectable in FORC diagrams (Muxworthy et al. 25). In such cases, other magnetic methods may be more suitable than FORC analysis. For example, in mixtures of MD magnetite and hematite, lowtemperature techniques can be more sensitive than FORC diagrams at identifying hematite in the presence of magnetite. (2) Source discrimination. Due to the detailed nature of FORC diagrams, they can be used to identify subtle differences between source materials that are not so readily observed using magnetic hysteresis data. For example, in a study of a loess/paleosol sequence from Moravia, two different source materials could be clearly distinguished and identified using FORC diagrams (van Oorschot et al. 22). There are many other apparent uses of FORC diagrams in environmental magnetic applications. (3) Assessing leaching. Sequential leaching techniques are commonly used by soil chemists to remove iron oxides from samples to facilitate clay mineral analysis. FORC analysis has been shown to help in elucidation of the leaching process where magnetic hysteresis alone was less diagnostic (Roberts et al. 2). (4) Preselection for paleointensity studies. In absolute paleointensity studies, SD assemblages should provide reliable results, while samples with strong magnetostatic interactions and/or MD grains should yield unacceptable results. Domain state and magnetostatic interactions are both readily identifiable on a FORC diagram, which should make them useful for sample screening and selection for absolute paleointensity studies. Likewise, strict criteria apply to the mineralogy, domain state and concentration of magnetic particles in sedimentary sequences in terms of their suitability for relative paleointensity studies. FORC diagrams therefore also have potential for screening sediments for relative paleointensity studies. Adrian R. Muxworthy and Andrew P. Roberts 9
10 1
11 Bibliography Day, R., Fuller, M. and Schmidt, V. A., Hysteresis properties of titanomagnetites: grainsize and compositional dependence. Physics of the Earth and Planetary Interiors, 13, Heslop, D. and Muxworthy, A. R., 25. Aspects of calculating firstorderreversalcurve distributions. Journal of Magnetism and Magnetic Materials, 288, Muxworthy, A. R., Heslop, D. and Williams, W., 24. Influence of magnetostatic interactions on firstorderreversalcurve (FORC) diagrams: a micromagnetic approach. Geophysical Journal International, 158, Muxworthy, A. R., King, J. G. and Heslop, D., 25. Assessing the ability of firstorder reversal curve (FORC) diagrams to unravel complex magnetic signals, Journal of Geophysical Research, 11, B115, doi:1.129/24jb3195. Muxworthy, A.R., Williams, W., and Virdee, D., 23. Effect of magnetostatic interactions on the hysteresis parameters of singledomain and pseudosingle domain grains, Journal of Geophysical Research, 18, B11, 2517, doi:1.129/23jb2588. Néel, L., Remarques sur la théorie des propriétés magnétiques des substances dures. Applied Scientific Research B, 4, Newell, A. J., 25. A highprecision model of firstorder reversal curve (FORC) functions for singledomain ferromagnets with uniaxial anisotropy. Geochemistry, Geophysics, Geosystems, 6, Q51, doi:1.129/24gc877. Pike, C. R., 23. Firstorder reversalcurve diagrams and reversible magnetization. Physics Review B, Pike, C. R., Roberts, A. P. and Verosub, K. L., Characterizing interactions in fine magnetic particle systems using first order reversal curves. Journal of Applied Physics, 85, Pike, C. R., Roberts, A. P., Dekkers, M. J. and Verosub, K. L., 21a. An investigation of multidomain hysteresis mechanisms using FORC diagrams, Physics of the Earth and Planetary Interiors, 126, Pike, C. R., Roberts, A. P. and Verosub, K. L., 21b. Firstorder reversal curve diagrams and thermal relaxation effects in magnetic particles, Geophysical Journal International, 145, Preisach, F., Über die magnetische Nachwirkung. Zeitschrift für Physik, 94, Roberts, A. P., Pike, C. R. and Verosub, K. L., 2. Firstorder reversal curve diagrams: a new tool for characterizing the magnetic properties of natural samples. Journal of Geophysical Research, 15, van Oorschot, I. H. M., Dekkers, M. J. and Havlicek, P., 22. Selective dissolution of magnetic iron oxides with the acid ammoniumoxalate/ferrousiron extraction technique  II. Natural loess and palaeosol samples. Geophysical Journal International, 149, Cross references Hysteresis 11
12 Figure captions Figure 1. Illustration of how FORC diagrams are constructed. (a) After applying a field at positive saturation (H SAT ), the field is reversed to H A and is then progressively increased at a range of H B values in the direction of H SAT. The magnetization is denoted by M(H A, H B ). The dashed line represents the major hysteresis loop and the solid line represents a single FORC. (b) A set of consecutive FORCs. (c) The M(H A, H B ) surface plotted in nonrotated field space (H A, H B ). (d) The resulting FORC diagram for the data shown in (b) and (c) for SF = 4. The FORC data shown in (b) to (d) are for a numerical model of randomly orientated uniaxial SD grains. Figure 2. (a) Schematic square hysteresis loop for an ideal noninteracting SD particle, with uniaxial anisotropy, aligned along the direction of the applied field (H SW is the switching field). (b) The raw hysteresis data for a series of FORCs for the grain shown in (a) plotted in nonrotated field space (H A, H B ). (c) FORC diagram for data shown in (a) and (b). The FORC distribution for this grain lies at H c = H SW and H u =. Figure 3. FORCs and FORC diagram for a numerical model of noninteracting 1 identical SD grains with randomly distributed uniaxial anisotropy (modified after Muxworthy et al. (24). The origins of the negative and positive regions in the FORC diagram are highlighted (SF = 4). The negative region is due to a decrease in M/ H B with decreasing H A for negative values of H B (H B1 ). The large positive peak is associated with the increase in M/ H B with decreasing H A for positive values of H B, near the switching field (H B2 ). The different return paths give rise the to the positive region of the FORC distribution to the right of the main peak as illustrated. Figure 4. FORC diagram (SF = 3; averaging time =.15 s) for an assemblage of noninteracting ideal SD grains for a tuff sample from Yucca Mountain, Nevada (from Roberts et al. (2). Figure 5. (a) Schematic diagram depicting the effect of a local interaction field H I on a square hysteresis loop for an ideal SD particle, with uniaxial anisotropy, aligned along the direction of the applied field, as shown in Fig. 2a. (b) Numerical simulation for an assemblage of 1 evenlyspaced, magnetitelike ideal SD grains with oriented uniaxial anisotropy. The distance between grains is 1.5 times the grains size. Figure 6. (a) FORC diagram (SF = 4; averaging time =.2 s) for a MD magnetite sample (mean grain size of 76 m). (b) FORC diagram (SF = 3; averaging time =.15 s) for a PSD magnetite sample (mean grain size of 1.7 m). (c) FORC diagram (SF = 3; averaging time = 12
13 .2 s) for tuff sample CS14 from Yucca Mountain, Nevada, containing SP magnetite (from Roberts et al. (2). Figure 7. Illustration of three methods for fitting a FORC diagram. (a) A truncated FORC diagram, with no extrapolation of data onto the H U axis; (b) a relaxedfit FORC diagram with extrapolation onto the H U axis; and (c) reversibleridge fitting (following Pike, 23). The sample is a PSD magnetite (mean grain size of.3 m; SF = 4; averaging time =.1s). Figure 8. (a) Major hysteresis loop and (b) FORC diagram for a sample containing PSD magnetite and PSD hematite in a ratio of 81:19. On the FORC diagram, the hematite is readily identified, but it is not evident in the major hysteresis loop (SF = 3; averaging time =.15 s). 13
14 (a) Measurement of a single FORC M (b) Raw FORC data M H SAT a single FORC M(H A,H B ) H H H A Major hysteresis loop (c) Raw FORC data in field space no measured data points + M s (d) A FORC diagram H A H A = H B M(H A,H B )  M s H B H U H B M(H A,H B ) a single FORC H C H B Figure 1 1
15 (a) Major hysteresis loop for a SD grain M ve H SW + ve H SW H (b) Rawdata hysteresis data plotted in fieldspace A single FORC + M s H A  M s H SW H B (c) FORC diagram for ideal SD grains H U H SW H C Figure 2 2
16 1 M H B2 2 M H A H B M w.r.t. H H A B rate of change of 44 M H B1 H B11 M H B2 2 M is positive H A H B2 4 H different return paths H U M H A H B1 is negative H C Figure 3 H U H C Figure 4 3
17 (a) M H I H H SW + H SW (b) 2 H u 11 spreading H c Figure 5 (a) MD (b) PSD (c) SP H u H c H c H c Figure 6 4
18 (a) Truncated diagram (b) Relaxedfit diagram (c) Reversibleridge diagram H u H c H c H c Figure 7 (a) M/M s H 1 (b) H U H C Figure 8 5
Firstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles
Click Here for Full Article JOURNAL OF GEOPHYSICAL RESEARCH, VOL. 112,, doi:10.1029/2006jb004575, 2007 Firstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles Amy
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationPreisach Models and FORC Diagrams: A Critical Appraisal from a Physicist's Perspective
Preisach Models and FORC Diagrams: A Critical Appraisal from a Physicist's Perspective R M. Roshko Department of Physics and Astronomy University of Manitoba Winnipeg, Manitoba, Canada First Order Reversal
More informationMagnetic Media Measurements with a VSM
Magnetic Media Measurements with a VSM B. C. Dodrill Lake Shore Cryotronics, Inc. 575 McCorkle Blvd Westerville, Ohio 43082 The last 50 years have seen the development of methods for the digital storage
More informationEM4: Magnetic Hysteresis
CHALMERS UNIVERSITY OF TECHNOLOGY GÖTEBORG UNIVERSITY EM4: Magnetic Hysteresis Lab manual (version 1.001a) Students:... &... Date:... /... /... Laboration passed:... Supervisor:... Date:... /... /... Raluca
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationMagnetic susceptibility and its variations with temperature, measuring field and operating frequency Examples from various rock types
Magnetic susceptibility and its variations with temperature, measuring field and operating frequency Examples from various rock types Identification of magnetic minerals and phases Grain size assessment
More informationHightemperature magnetic stability of small magnetite particles
JOURNAL OF GEOPHYSICAL RESEARCH, VOL. 108, NO. B5, 2281, doi:10.1029/2002jb002195, 2003 Hightemperature magnetic stability of small magnetite particles Adrian R. Muxworthy 1 and David J. Dunlop Geophysics,
More informationAppendix E: Graphing Data
You will often make scatter diagrams and line graphs to illustrate the data that you collect. Scatter diagrams are often used to show the relationship between two variables. For example, in an absorbance
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationAP Physics 1 and 2 Lab Investigations
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
More informationIN current film media, the increase in areal density has
IEEE TRANSACTIONS ON MAGNETICS, VOL. 44, NO. 1, JANUARY 2008 193 A New Read Channel Model for Patterned Media Storage Seyhan Karakulak, Paul H. Siegel, Fellow, IEEE, Jack K. Wolf, Life Fellow, IEEE, and
More informationThe accurate calibration of all detectors is crucial for the subsequent data
Chapter 4 Calibration The accurate calibration of all detectors is crucial for the subsequent data analysis. The stability of the gain and offset for energy and time calibration of all detectors involved
More information2. Permanent Magnet (De) Magnetization 2.1 Methodology
Permanent Magnet (De) Magnetization and Soft Iron Hysteresis Effects: A comparison of FE analysis techniques A.M. Michaelides, J. Simkin, P. Kirby and C.P. Riley Cobham Technical Services Vector Fields
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationThe interaction of Cu(100)Fe surfaces with oxygen studied with photoelectron spectroscopy. I
5 The interaction of Cu(100)Fe surfaces with oxygen studied with photoelectron spectroscopy. I Mg Kα excited photoemission. Abstract The oxidation of Cu(100)Fe surfaces was studied using XPS. Surfaces
More informationChapter 4. Magnetic Materials and Circuits
Chapter 4 Magnetic Materials and Circuits Objectives List six characteristics of magnetic field. Understand the righthand rule for current and magnetic fluxes. Define magnetic flux, flux density, magnetomotive
More informationEðlisfræði 2, vor 2007
[ Assignment View ] [ Pri Eðlisfræði 2, vor 2007 28. Sources of Magnetic Field Assignment is due at 2:00am on Wednesday, March 7, 2007 Credit for problems submitted late will decrease to 0% after the deadline
More informationNonlinear Iterative Partial Least Squares Method
Numerical Methods for Determining Principal Component Analysis Abstract Factors Béchu, S., RichardPlouet, M., Fernandez, V., Walton, J., and Fairley, N. (2016) Developments in numerical treatments for
More informationMy lecture slides are posted at Information for Physics 112 midterm, Wednesday, May 2
My lecture slides are posted at http://www.physics.ohiostate.edu/~humanic/ Information for Physics 112 midterm, Wednesday, May 2 1) Format: 10 multiple choice questions (each worth 5 points) and two showwork
More informationNew Approach to Analysis of the Switching Current Data in Ferroelectric Thin Films
Ferroelectrics, 291: 27 35, 2003 Copyright c Taylor & Francis Inc. ISSN: 00150193 print / 15635112 online DOI: 10.1080/00150190390222510 New Approach to Analysis of the Switching Current Data in Ferroelectric
More informationQNET Experiment #06: HVAC Proportional Integral (PI) Temperature Control Heating, Ventilation, and Air Conditioning Trainer (HVACT)
Quanser NIELVIS Trainer (QNET) Series: QNET Experiment #06: HVAC Proportional Integral (PI) Temperature Control Heating, Ventilation, and Air Conditioning Trainer (HVACT) Student Manual Table of Contents
More informationMathematics 31 Precalculus and Limits
Mathematics 31 Precalculus and Limits Overview After completing this section, students will be epected to have acquired reliability and fluency in the algebraic skills of factoring, operations with radicals
More informationChapter 8. Low energy ion scattering study of Fe 4 N on Cu(100)
Low energy ion scattering study of 4 on Cu(1) Chapter 8. Low energy ion scattering study of 4 on Cu(1) 8.1. Introduction For a better understanding of the reconstructed 4 surfaces one would like to know
More informationEXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION
EXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION Hua Yuan and David E. Laughlin Department of Materials Science and Engineering, Carnegie Mellon
More informationChapter 6: Constructing and Interpreting Graphic Displays of Behavioral Data
Chapter 6: Constructing and Interpreting Graphic Displays of Behavioral Data Chapter Focus Questions What are the benefits of graphic display and visual analysis of behavioral data? What are the fundamental
More informationCopyright 2007 Casa Software Ltd. www.casaxps.com. ToF Mass Calibration
ToF Mass Calibration Essentially, the relationship between the mass m of an ion and the time taken for the ion of a given charge to travel a fixed distance is quadratic in the flight time t. For an ideal
More informationA Strategy for Teaching Finite Element Analysis to Undergraduate Students
A Strategy for Teaching Finite Element Analysis to Undergraduate Students Gordon Smyrell, School of Computing and Mathematics, University of Teesside The analytical power and design flexibility offered
More informationIncorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
The OpenAccess Journal for the Basic Principles of Diffusion Theory, Experiment and Application Incorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
More informationPermanent Magnet Materials
Measurements with a VSM Permanent Magnet Materials B. C. Dodrill B. J. Kelley Lake Shore Cryotronics, Inc. 575 McCorkle Blvd. Westerville, OH, 43082 Please address correspondence to bdodrill@lakeshore.com
More informationUsing Excel (Microsoft Office 2007 Version) for Graphical Analysis of Data
Using Excel (Microsoft Office 2007 Version) for Graphical Analysis of Data Introduction In several upcoming labs, a primary goal will be to determine the mathematical relationship between two variable
More informationAn octave bandwidth dipole antenna
An octave bandwidth dipole antenna Abstract: Achieving wideband performance from resonant structures is challenging because their radiation properties and impedance characteristics are usually sensitive
More informationReview of Fundamental Mathematics
Review of Fundamental Mathematics As explained in the Preface and in Chapter 1 of your textbook, managerial economics applies microeconomic theory to business decision making. The decisionmaking tools
More informationFall 12 PHY 122 Homework Solutions #8
Fall 12 PHY 122 Homework Solutions #8 Chapter 27 Problem 22 An electron moves with velocity v= (7.0i  6.0j)10 4 m/s in a magnetic field B= (0.80i + 0.60j)T. Determine the magnitude and direction of the
More informationOptiffuser. Highperformance, high bandwidth lightweight 1D diffuser.
Optiffuser Highperformance, high bandwidth lightweight 1D diffuser. General product information The Optiffuser comes in packs of four panels. Two positives and two negatives (see page 5) per package.
More informationPiezo Technologies  Technical Resource Paper
in Piezoceramic Materials One can think of a piezoceramic as a rock which generates electrical current if squeezed and which moves if driven by an electrical current. For these wonderful properties to
More informationChapter 19: Magnetic Forces and Fields
Chapter 19: Magnetic Forces and Fields Magnetic Fields Magnetic Force on a Point Charge Motion of a Charged Particle in a Magnetic Field Crossed E and B fields Magnetic Forces on Current Carrying Wires
More informationMetamorphic rocks are rocks changed from one form to another by intense heat, intense pressure, and/or the action of hot fluids.
Metamorphic Rocks, Processes, and Resources Metamorphic rocks are rocks changed from one form to another by intense heat, intense pressure, and/or the action of hot fluids. Protolith or parent rock is
More informationMotorCAD Software for Thermal Analysis of Electrical Motors  Links to Electromagnetic and Drive Simulation Models
MotorCAD Software for Thermal Analysis of Electrical Motors  Links to Electromagnetic and Drive Simulation Models Dave Staton, Douglas Hawkins and Mircea Popescu Motor Design Ltd., Ellesmere, Shropshire,
More informationFirstorder reversal curve (FORC) diagrams for pseudosingledomain magnetites at high temperature
Earth and Planetary Science Letters 203 (2002) 369^382 www.elsevier.com/locate/epsl Firstorder reversal curve (FORC) diagrams for pseudosingledomain magnetites at high temperature Adrian R. Muxworthy,David
More informationPhysics 112 Homework 5 (solutions) (2004 Fall) Solutions to Homework Questions 5
Solutions to Homework Questions 5 Chapt19, Problem2: (a) Find the direction of the force on a proton (a positively charged particle) moving through the magnetic fields in Figure P19.2, as shown. (b) Repeat
More informationMA 323 Geometric Modelling Course Notes: Day 02 Model Construction Problem
MA 323 Geometric Modelling Course Notes: Day 02 Model Construction Problem David L. Finn November 30th, 2004 In the next few days, we will introduce some of the basic problems in geometric modelling, and
More informationCommon Tools for Displaying and Communicating Data for Process Improvement
Common Tools for Displaying and Communicating Data for Process Improvement Packet includes: Tool Use Page # Box and Whisker Plot Check Sheet Control Chart Histogram Pareto Diagram Run Chart Scatter Plot
More informationBoltzmann Distribution Law
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
More informationReflection and Refraction
Equipment Reflection and Refraction Acrylic block set, planeconcaveconvex universal mirror, cork board, cork board stand, pins, flashlight, protractor, ruler, mirror worksheet, rectangular block worksheet,
More informationAnomalous Hall Effect Magnetometry A Method for Studying Magnetic Processes of Thin Magnetic Films
Anomalous Hall Effect Magnetometry A Method for Studying Magnetic Processes of Thin Magnetic Films J. R. Lindemuth a, B. C. Dodrill a and N. C. Oldham b a Lake Shore Cryotronics, Inc. 575 McCorkle Blvd,
More informationIron Powder Cores for Switchmode Power Supply Inductors. by: Jim Cox
HOME APPLICATION NOTES Iron Powder Cores for Switchmode Power Supply Inductors by: Jim Cox Purpose: The purpose of this application note is to cover the properties of iron powder as a magnetic core material
More informationSixstate, threelevel, sixfold ferromagnetic wire system
Sixstate, threelevel, sixfold ferromagnetic wire system T. Blachowicz 1a and A. Ehrmann 2 1 Institute of Physics, Silesian University of Technology, 44100 Gliwice, Poland 2 Faculty of Textile and Clothing
More informationExperiment #1, Analyze Data using Excel, Calculator and Graphs.
Physics 182  Fall 2014  Experiment #1 1 Experiment #1, Analyze Data using Excel, Calculator and Graphs. 1 Purpose (5 Points, Including Title. Points apply to your lab report.) Before we start measuring
More informationPOISSON AND LAPLACE EQUATIONS. Charles R. O Neill. School of Mechanical and Aerospace Engineering. Oklahoma State University. Stillwater, OK 74078
21 ELLIPTICAL PARTIAL DIFFERENTIAL EQUATIONS: POISSON AND LAPLACE EQUATIONS Charles R. O Neill School of Mechanical and Aerospace Engineering Oklahoma State University Stillwater, OK 74078 2nd Computer
More informationCHAPTER 5: MAGNETIC PROPERTIES
CHAPTER 5: MAGNETIC PROPERTIES and Magnetic Materials ISSUES TO ADDRESS... Why do we study magnetic properties? What is magnetism? How do we measure magnetic properties? What are the atomic reasons for
More informationApplication of Stop and Play Models to the Representation of Magnetic Characteristics of Silicon Steel Sheet
Title Application of stop and play models magnetic characteristics of silicon Author(s) Matsuo, T; Shimode, D; Terada, Y; S Citation IEEE TRANSACTIONS ON MAGNETICS (200 13611364 Issue Date 200305 URL
More informationDetermination of g using a spring
INTRODUCTION UNIVERSITY OF SURREY DEPARTMENT OF PHYSICS Level 1 Laboratory: Introduction Experiment Determination of g using a spring This experiment is designed to get you confident in using the quantitative
More informationSputtering by Particle Bombardment I
Sputtering by Particle Bombardment I Physical Sputtering of SingleElement Solids Edited by R. Behrisch With Contributions by H. H. Andersen H. L. Bay R. Behrisch M. T. Robinson H. E. Roosendaal P. Sigmund
More informationUniversity Turbine Systems Research 2012 Fellowship Program Final Report. Prepared for: General Electric Company
University Turbine Systems Research 2012 Fellowship Program Final Report Prepared for: General Electric Company Gas Turbine Aerodynamics Marion Building 300 Garlington Rd Greenville, SC 29615, USA Prepared
More informationInsertion Devices Lecture 4 Permanent Magnet Undulators. Jim Clarke ASTeC Daresbury Laboratory
Insertion Devices Lecture 4 Permanent Magnet Undulators Jim Clarke ASTeC Daresbury Laboratory Introduction to Lecture 4 So far we have discussed at length what the properties of SR are, when it is generated,
More informationClassification of Fingerprints. Sarat C. Dass Department of Statistics & Probability
Classification of Fingerprints Sarat C. Dass Department of Statistics & Probability Fingerprint Classification Fingerprint classification is a coarse level partitioning of a fingerprint database into smaller
More informationInterpreting Data in Normal Distributions
Interpreting Data in Normal Distributions This curve is kind of a big deal. It shows the distribution of a set of test scores, the results of rolling a die a million times, the heights of people on Earth,
More informationSimulation of Residual Stresses in an Induction Hardened Roll
2.6.4 Simulation of Residual Stresses in an Induction Hardened Roll Ludwig Hellenthal, Clemens Groth Walzen Irle GmbH, NetphenDeuz, Germany CADFEM GmbH, Burgdorf/Hannover, Germany Summary A heat treatment
More information2D Magnetic Circuit Analysis for a Permanent Magnet Used in Laser Ablation Plume Expansion Experiments
University of California, San Diego UCSDLPLM0204 2D Magnetic Circuit Analysis for a Permanent Magnet Used in Laser Ablation Plume Expansion Experiments Xueren Wang, Mark Tillack and S. S. Harilal December
More informationFlorida Math for College Readiness
Core Florida Math for College Readiness Florida Math for College Readiness provides a fourthyear math curriculum focused on developing the mastery of skills identified as critical to postsecondary readiness
More informationGas Dynamics Prof. T. M. Muruganandam Department of Aerospace Engineering Indian Institute of Technology, Madras. Module No  12 Lecture No  25
(Refer Slide Time: 00:22) Gas Dynamics Prof. T. M. Muruganandam Department of Aerospace Engineering Indian Institute of Technology, Madras Module No  12 Lecture No  25 PrandtlMeyer Function, Numerical
More informationFILTER CIRCUITS. A filter is a circuit whose transfer function, that is the ratio of its output to its input, depends upon frequency.
FILTER CIRCUITS Introduction Circuits with a response that depends upon the frequency of the input voltage are known as filters. Filter circuits can be used to perform a number of important functions in
More informationHigh Resolution Spatial Electroluminescence Imaging of Photovoltaic Modules
High Resolution Spatial Electroluminescence Imaging of Photovoltaic Modules Abstract J.L. Crozier, E.E. van Dyk, F.J. Vorster Nelson Mandela Metropolitan University Electroluminescence (EL) is a useful
More informationChapter 2. Derivation of the Equations of Open Channel Flow. 2.1 General Considerations
Chapter 2. Derivation of the Equations of Open Channel Flow 2.1 General Considerations Of interest is water flowing in a channel with a free surface, which is usually referred to as open channel flow.
More informationHow to Win the Stock Market Game
How to Win the Stock Market Game 1 Developing ShortTerm Stock Trading Strategies by Vladimir Daragan PART 1 Table of Contents 1. Introduction 2. Comparison of trading strategies 3. Return per trade 4.
More informationPlate Tectonics: Ridges, Transform Faults and Subduction Zones
Plate Tectonics: Ridges, Transform Faults and Subduction Zones Goals of this exercise: 1. review the major physiographic features of the ocean basins 2. investigate the creation of oceanic crust at midocean
More informationThe successful integration of 3D seismic into the mining process: Practical examples from Bowen Basin underground coal mines
Geophysics 165 Troy Peters The successful integration of 3D seismic into the mining process: Practical examples from Bowen Basin underground coal mines This paper discusses how mine staff from a number
More informationMeasurement of Specific Heat Capacity Using Differential Scanning Calorimeter
INL/EXT0815056 Measurement of Specific Heat Capacity Using Differential Scanning Calorimeter J. E. Daw November 2008 The INL is a U.S. Department of Energy National Laboratory operated by Battelle Energy
More informationThe dream for a better life has made man look for gold coins from the World War II (1940) which were lost in various parts of Greece.
The search for gold and gold coins is one of the finest and the most widespread hobbies. It has its difficulties as well as its beautiful moments. The people involved in this hobby are commonly called
More informationMap Patterns and Finding the Strike and Dip from a Mapped Outcrop of a Planar Surface
Map Patterns and Finding the Strike and Dip from a Mapped Outcrop of a Planar Surface Topographic maps represent the complex curves of earth s surface with contour lines that represent the intersection
More informationAtomic Force Microscope and Magnetic Force Microscope Background Information
Atomic Force Microscope and Magnetic Force Microscope Background Information Lego Building Instructions There are several places to find the building instructions for building the Lego models of atomic
More informationKOLEKTOR MAGNET TECHNOLOGY
ZIT S KOERZIT S Sintered AlNiCo Koerzit is the KOLEKTOR MAGNET TECHNOLOGY GmbH tradename for sintered permanent magnets based on AlNi and AlNiCo alloys. Koerzit magnets are made by powder metallurgy. KOLEKTOR
More informationE/M Experiment: Electrons in a Magnetic Field.
E/M Experiment: Electrons in a Magnetic Field. PRELAB You will be doing this experiment before we cover the relevant material in class. But there are only two fundamental concepts that you need to understand.
More informationAssignment #3: Plate Tectonics
Assignment #3: Plate Tectonics Overview: In this assignment we will examine the ideas of continental drift and of seafloor spreading that lead to the Theory of Plate Tectonics. This assignment is in two
More informationMIKE 21 FLOW MODEL HINTS AND RECOMMENDATIONS IN APPLICATIONS WITH SIGNIFICANT FLOODING AND DRYING
1 MIKE 21 FLOW MODEL HINTS AND RECOMMENDATIONS IN APPLICATIONS WITH SIGNIFICANT FLOODING AND DRYING This note is intended as a general guideline to setting up a standard MIKE 21 model for applications
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationAn Analysis of the Rossby Wave Theory
An Analysis of the Rossby Wave Theory Morgan E. Brown, Elise V. Johnson, Stephen A. Kearney ABSTRACT Largescale planetary waves are known as Rossby waves. The Rossby wave theory gives us an idealized
More informationDevelopment of HighPerformance ASVLCDs Using Continuous Pinwheel Alignment (CPA) Mode
Development of HighPerformance ASVLCDs Using Continuous Pinwheel Alignment (CPA) Mode Masumi Kubo * Toshihiko Miyashita *2 Nobuyoshi Nagashima *3 Eiichiroh Nishimura *4 * A30 Project Team, TFT Liquid
More informationPATHOGEN DETECTION SYSTEMS BY REAL TIME PCR. Results Interpretation Guide
PATHOGEN DETECTION SYSTEMS BY REAL TIME PCR Results Interpretation Guide Pathogen Detection Systems by Real Time PCR Microbial offers real time PCR based systems for the detection of pathogenic bacteria
More informationAuxiliary material for Paper 2004JE002305R Shock Properties of H 2 OIce
Auxiliary material for Paper 2004JE002305R Shock Properties of H 2 OIce 1 Sarah T. Stewart* and Thomas J. Ahrens Lindhurst Laboratory of Experimental Geophysics, California Institute of Technology, Pasadena,
More informationState of Stress at Point
State of Stress at Point Einstein Notation The basic idea of Einstein notation is that a covector and a vector can form a scalar: This is typically written as an explicit sum: According to this convention,
More informationEXPONENTS. To the applicant: KEY WORDS AND CONVERTING WORDS TO EQUATIONS
To the applicant: The following information will help you review math that is included in the Paraprofessional written examination for the Conejo Valley Unified School District. The Education Code requires
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationCommon Core Unit Summary Grades 6 to 8
Common Core Unit Summary Grades 6 to 8 Grade 8: Unit 1: Congruence and Similarity 8G18G5 rotations reflections and translations,( RRT=congruence) understand congruence of 2 d figures after RRT Dilations
More informationMaster in Earth Sciences
Master in Earth Sciences DERDW EARTH SCIENCES MASTER IN EARTH SCIENCES The Department of Earth Sciences at ETH Zurich has been repeatedly ranked as one of the world s leading Earth Science schools. The
More informationAlgebra 1 Course Information
Course Information Course Description: Students will study patterns, relations, and functions, and focus on the use of mathematical models to understand and analyze quantitative relationships. Through
More informationIncreasing for all. Convex for all. ( ) Increasing for all (remember that the log function is only defined for ). ( ) Concave for all.
1. Differentiation The first derivative of a function measures by how much changes in reaction to an infinitesimal shift in its argument. The largest the derivative (in absolute value), the faster is evolving.
More informationStress and deformation of offshore piles under structural and wave loading
Stress and deformation of offshore piles under structural and wave loading J. A. Eicher, H. Guan, and D. S. Jeng # School of Engineering, Griffith University, Gold Coast Campus, PMB 50 Gold Coast Mail
More information1 Error in Euler s Method
1 Error in Euler s Method Experience with Euler s 1 method raises some interesting questions about numerical approximations for the solutions of differential equations. 1. What determines the amount of
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationCORRELATED TO THE SOUTH CAROLINA COLLEGE AND CAREERREADY FOUNDATIONS IN ALGEBRA
We Can Early Learning Curriculum PreK Grades 8 12 INSIDE ALGEBRA, GRADES 8 12 CORRELATED TO THE SOUTH CAROLINA COLLEGE AND CAREERREADY FOUNDATIONS IN ALGEBRA April 2016 www.voyagersopris.com Mathematical
More informationAmpere's Law. Introduction. times the current enclosed in that loop: Ampere's Law states that the line integral of B and dl over a closed path is 0
1 Ampere's Law Purpose: To investigate Ampere's Law by measuring how magnetic field varies over a closed path; to examine how magnetic field depends upon current. Apparatus: Solenoid and path integral
More informationXRay Study of Soft and Hard Magnetic Thin Films
Copyright (C) JCPDSInternational Centre for Diffraction Data 1999 13 XRay Study of Soft and Hard Magnetic Thin Films PoWen Wang, 390 Reed St., Stormedia, Inc., Santa Clara CA. 95050 Abstract : This
More informationE. K. A. ADVANCED PHYSICS LABORATORY PHYSICS 3081, 4051 NUCLEAR MAGNETIC RESONANCE
E. K. A. ADVANCED PHYSICS LABORATORY PHYSICS 3081, 4051 NUCLEAR MAGNETIC RESONANCE References for Nuclear Magnetic Resonance 1. Slichter, Principles of Magnetic Resonance, Harper and Row, 1963. chapter
More information11.1. Objectives. Component Form of a Vector. Component Form of a Vector. Component Form of a Vector. Vectors and the Geometry of Space
11 Vectors and the Geometry of Space 11.1 Vectors in the Plane Copyright Cengage Learning. All rights reserved. Copyright Cengage Learning. All rights reserved. 2 Objectives! Write the component form of
More information2.500 Threshold. 2.000 1000e  001. Threshold. Exponential phase. Cycle Number
application note RealTime PCR: Understanding C T RealTime PCR: Understanding C T 4.500 3.500 1000e + 001 4.000 3.000 1000e + 000 3.500 2.500 Threshold 3.000 2.000 1000e  001 Rn 2500 Rn 1500 Rn 2000
More informationCHAPTER 6 THE TERRESTRIAL PLANETS
CHAPTER 6 THE TERRESTRIAL PLANETS MULTIPLE CHOICE 1. Which of the following is NOT one of the four stages in the development of a terrestrial planet? 2. That Earth, evidence that Earth differentiated.
More informationAnamorphic imaging with three mirrors: a survey
Anamorphic imaging with three mirrors: a survey Joseph M. Howard Optics Branch (Code 551), NASA Goddard Space Flight Center, Greenbelt, MD 20771 Ph: 3012860690 Fax: 3012860204 Joseph.M.Howard@nasa.gov
More informationDC GENERATOR THEORY. LIST the three conditions necessary to induce a voltage into a conductor.
DC Generators DC generators are widely used to produce a DC voltage. The amount of voltage produced depends on a variety of factors. EO 1.5 LIST the three conditions necessary to induce a voltage into
More information